This is a repository copy of Shrinkage and flexural behaviour of free and restrained hybrid steel fibre reinforced concrete.
White Rose Research Online URL for this paper: http://eprints.whiterose.ac.uk/154396/
Version: Accepted Version
Al-Kamyani, Z., Figueiredo, F.P., Hu, H. et al. (2 more authors) (2018) Shrinkage and flexural behaviour of free and restrained hybrid steel fibre reinforced concrete.
Construction and Building Materials, 189. pp. 1007-1018. ISSN 0950-0618 https://doi.org/10.1016/j.conbuildmat.2018.09.052
Article available under the terms of the CC-BY-NC-ND licence (https://creativecommons.org/licenses/by-nc-nd/4.0/).
This article is distributed under the terms of the Creative Commons Attribution-NonCommercial-NoDerivs (CC BY-NC-ND) licence. This licence only allows you to download this work and share it with others as long as you credit the authors, but you can’t change the article in any way or use it commercially. More
information and the full terms of the licence here: https://creativecommons.org/licenses/
If you consider content in White Rose Research Online to be in breach of UK law, please notify us by
Shrinkage and Flexural Behaviour of Free and Restrained Hybrid Steel Fibre1
The effect of restrained shrinkage on the mechanical performance of concrete and steel
fibre reinforced concrete (SFRC) requires more investigation, especially when using recycled
tyre steel fibre (RTSF). This paper examines the free and restrained shrinkage strains and the
mechanical performance of seven SFRC mixes. Results show that both free and restrained
average shrinkage strains are very similar in all blends of fibres and they exhibited
uniform shrinkage through the height of the section. All examined blends meet strength
requirements by MC-2010 for fibres to replace part of the conventional reinforcement in RC
Free shrinkage strains are not affected significantly by addition of steel fibres.
GGBS reduces shrinkage strains.
Recycled tyre steel fibres can replace manufactured steel fibres partially.
In water retaining structures or bridge elements, serviceability limit state (SLS) design
aims to control crack widths to achieve a target life span by providing relatively large
amounts of surface steel reinforcement. In such structures, the additional reinforcement is
required to control cracks induced by restrained shrinkage, which creates further
constructability challenges. To reduce the amount of additional surface reinforcement,
shrinkage can be mitigated by reducing paste/aggregate ratio, minimising C3S content in 22
cement, using expansive or shrinkage reducing additives, and internal curing materials .
Shrinkage cracking can also be controlled by adding randomly distributed steel fibres as
successfully utilised by the construction industry in pavements and tunnels [2, 3, 4]. Steel
fibres can enhance the performance of concrete in flexure, shear and punching whilst at the
same time help control shrinkage cracking and reduce spalling [5, 6, 7], depending on the
amount and characteristics of the steel fibres, such as type, shape and aspect ratio [8, 9, 10,
11]. Recycled tyre steel fibres (RTSF) are also available and were found to be good in
controlling micro-cracks [12, 8]. RTSF can improve flexural toughness and post cracking
performance and can successfully substitute manufactured fibres partially or fully in some
applications [9, 13].
In most published research on RTSF [4, 14, 15], a single type of fibre is used as
reinforcement. Recently, some studies investigated blends of manufactured and recycled steel
fibres with different shapes and aspect ratios [9, 16], but the recycled fibres used were not
classified raising reliability and repeatability concerns. The cleaning process of RTSF has
been improved significantly recently and improved classified fibres have become available
[17, 18, 19]. Hence, there is a need to investigate the effect of hybrid steel fibres (both
manufactured and classified RTSF) on concrete exposed to free and restrained shrinkage.
The impact of steel fibres on free shrinkage of concrete is not clearly understood, with
some researchers reporting an increase due to the increase in air voids, whilst others reporting
either a decrease due to the internal restraint provided by the fibres or insignificant changes
due to the cancelling effect of the two actions [4, 14, 15, 20]. Nonetheless, the effect of steel
fibres on free shrinkage is known to vary depending on water-to-binder ratio, volume and
type of admixtures, method of concrete laying (conventional, self-compacted concrete (SCC)
or roller compacted concrete (RCC)), time of vibration, etc. .
In concrete structures, shrinkage of concrete is restrained by different actions internally
and externally. External restraint can arise due to friction or reaction against the ground,
concrete supporting elements or adjacent rigid structures, whilst internal restraint is provided
by aggregates and reinforcement [22, 23]. It is also known that aggregates tend to settle and
concentrate at the bottom of the mould whilst water and air rise due to vibration and surface
tamping. These phenomena can cause differences in compressive strength and elastic
modulus at the top and bottom of the element [24, 25]. As more paste and water are found
near the top surface, this can cause much higher shrinkage strains in that region. Non-uniform
distribution of aggregates and water can create non-uniform shrinkage through a section and
lead to additional curvature in concrete elements . RILEM TC 107-CSP  determines
shrinkage from the change in the distance between the centres of the two ends of a cylinder,
which means that its approach is unable to capture the effect of aggregate sedimentation. To
the knowledge of the authors, none of the design codes or standards deal with curvature due
to the non-uniform shrinkage and this can lead to underestimate of long-term deflections and
Free shrinkage tests on small elements are not normally able to develop enough internal
tensile stresses to crack the concrete, hence, restrained shrinkage tests are needed to
understand the cracking behaviour of restrained concrete . Restraint causes tensile
stresses in the concrete, which theoretically could increase with time due to concrete
maturity, but creep is expected to relieve some of these stresses and reduce the probability of
cracking [23, 27, 28]. Normally, it is difficult to quantify the degree of restraint imposed on
an element, as it depends on the type of application, the location of the member in the
structure and environmental conditions [3, 29]. However, there are several tests to assess the
restrained shrinkage of concrete , with the most used being the ring test [30, 31]. Though
simple and popular, this test can only be used for comparison purposes, as it only detects the
stress and time of the first crack. Another disadvantage of this approach is that the sectional
size needs to be kept relatively small (to enable cracking at a reasonable time frame) and this
enhances boundary effects and makes the concrete section less representative of sections in
Active systems with larger specimens [32, 33, 34] can be used to restrain concrete
shrinkage by fixing one end of a linear element whilst the other end is attached to an actuator
which keeps the total length constant. In active systems, cracks tend to occur when the strain
is being adjusted and this can affect the time at which cracking takes place . Furthermore,
full and active restrain is rarely found in practice, where restrain depends on the relative
stiffness of the restraining structure and is mitigated by creep. For these reasons, and for
simplicity, passive systems [36, 37] can be used by restraining concrete specimens through
fixing bolts onto rigid structural elements. Younis (2014)  proposed the use of a passive
restraining frame able to hold three prisms at the same time. The use of linear elements also
enables shrinkage measurements to be taken at different levels through the section and
examine shrinkage curvature.
The aim of this work is to examine the effect of restrain on shrinkage and mechanical
performance of hybrid SFRC mixes. The performance of SFRC prisms comprising different
fibre blends and subjected to a combination of restraining, curing and drying conditions are
studied and compared. Ground granulated blast-furnace slag (GGBS) and RTSF are used,
along with manufactured fibres, to control the amount of shrinkage strains and limit the
propagation of concrete cracking under restrained conditions.
This paper comprises three main sections along with an introduction and conclusions.
The first section presents the experimental programme including the examined parameters,
the physical and mechanical characteristics of the examined materials and testing
methodology. This is followed by a discussion on the results obtained from free and
restrained shrinkage tests of hybrid SFRC prisms (blends of manufactured undulated steel
fibres (MUSF) and RTSF). The level of restrain imposed by restraining frames is assessed
through a finite element numerical analysis and used to gain additional insight into the effect
of restraint level on overall behaviour. Finally, in the third section the paper discusses the
effect of restrained shrinkage and different drying conditions on the flexural performance of
the examined concrete mixes.
2. Experimental Programme
The experimental programme examined seven SFRC mixes in addition to a control mix
made of plain concrete, as shown in Table 1. Each mix was used to manufacture twelve
control cubes (100 mm), six prisms (100x100x500mm) for free shrinkage measurement and
three prisms, which were cast in a restraining steel frame as shown in Figure 1a . Three
prisms (out of the six) were stored in a mist room (MR) to monitor autogenous shrinkage.
The other three specimens were stored under controlled environmental (CR) conditions
(temp: 23±2 °C and RH: 40±5%) to quantify drying shrinkage. The restrained specimens
(RS) were stored under the same conditions as the CR specimens.
Table 1 Steel fibre types and contents. 113 Mix MUSF L (mm) MUSF Ø (mm) MUSF Dose (kg/m3) RTSF Dose (kg/m3) RTPF Dose (kg/m3) Batch number P - - - 1, 2, 3 M30 55 0.8 30 - - 1 M20R10 55 0.8 20 10 - 2 M20R10P1 55 0.8 20 10 1 3 R30 - - - 30 - 3 M35 60 1.0 35 - - 1 M45 60 1.0 45 - - 1 M35R10 60 1.0 35 10 - 2 114
Figure 1 Restraining frame used to restrain concrete prisms (a) and layout of shrinkage DEMEC distribution in free (b) and 115 restrained prisms (c). 116 117 2.2 Measurements 118
Shrinkage measurements were taken using a 200-mm demountable mechanical
“DEMEC” strain gauge at the top and bottom of both sides of all prisms for 300 days. Figure
1 (b and c) shows the measurement layout for free and restrained shrinkage, respectively. It
should be noted that a 100 mm “DEMEC” strain gauge was used to measure the deformation
at the boundaries between concrete and restraining frame.
At the end of the shrinkage measurement period, CR prisms were dried in an oven until
constant weight was observed. This was always achieved after les at 0 C and les
at 100 C, each cycle lasting 24 hours. After that and prior to flexural testing, all prisms were
notched (on one of the sides as cast) at the centre to 1/6 of the sectional depth. They were
then tested in three-point flexure by controlling the crack mouth opening displacement
*All dimensions are in mm *Sketch is not to scale
(CMOD) . The exact dimensions of the prisms were taken to the nearest 0.5 mm to
account for casting imperfections. Each prism was then split into two pieces and each portion
tested for compressive strength according to BS 1881-119 . Concrete compressive
strength was also obtained from cube test at 7 days, 28 days and 14 months.
Two types of steel fibres were used in this programme: manufactured undulated fibres
(MUSF) with a nominal tensile strength of 1450 MPa (two types of undulated
length/diameter (L/Ø) 55/0.8 and 60/1) and recycled tyre steel fibres (RTSF) with a nominal
tensile strength greater than 2000 MPa . The average diameter of RTSF was about 0.2
mm, whilst the average length, determined using a special optical device, at 50% cumulative
mass, was about 20 mm as shown in Figure 2. Both single and blended steel fibres were used
to reinforce the concrete in three amounts of 30 kg/m3, 35 kg/m3 or 45 kg/m3. Mix
M20R10P1 also contained 1 kg/m3 of recycled tyre polymer fibres (RTPF) to examine the
effect of polymer fibres in controlling shrinkage cracking.
Figure 2 Length distribution of classified RTSF. 144
Three batches of ready mix concrete were used to manufacture the test specimens (see
Table 2). The mix design is based on a design used in Europe for slabs-on-grade. The binder
consisted of 50% CEM 1 and 50% GGBS.
8 Table 2 Nominal mix composition.
149 Composition Quantity (kg/m3) Cement 52.5N CEM1 150 GGBS (BS EN 15167-1:2006) 150 4/20 River aggregates 1097 0/4 River sand 804 Water/binder ratio 0.55 SP (Master Polyheed 410) 1.5 L 150
3. Results and Discussion on Shrinkage Strains
3.1Free shrinkage strains
3.1.1 Drying shrinkage
The free shrinkage strains versus time at the top and bottom of the specimen (T for top
and B for bottom) are shown in Figure 3 (a and b), respectively. The small fluctuations in the
curves are a result of small temperature and relative humidity changes in the control room.
Shrinkage strain predictions of Eurocode  and fib Model Code , shown in dotted
lines, are higher than the experimental strains, possibly due to the high amount of GGBS and
differences in first measurement time. The EC and fib models consider conventional cements
and do not consider other cementitious materials in their predictions. GGBS was found by
some authors to reduce total shrinkage amount (average of top and bottom measurement) [35,
43, 44] as the fineness of GGBS can close the concrete pores and prevent water from
escaping the substrate . Codes recommend taking the first shrinkage measurements
within 3 minutes after demoulding, but due to the high amount of DEMEC discs used in this
study, the first shrinkage measurement was taken after 6 hours.
Figure 3 Free shrinkage strains at top (a) and bottom (b). 166
It is difficult to determine, from the results, the precise effect of steel fibre type/dosage
on free shrinkage. However, it is evident that shrinkage strains at the top are overall higher
than at the bottom possibly due to non-uniform distribution of concrete constituents. Plain
concrete shows higher shrinkage strains at the top than SFRC mixes, whilst showing the
lowest strain at the bottom. This may be due to the fact that superplasticiser was added to the
172 0 100 200 300 400 500 600 700 800 0 50 100 150 200 250 300 S h rin k a g e (m icr o -str a in s) Age (days) M30T M20R10T M20R10P1T R30T M35T M45T M35R10T PT MC-10 EC (a) 0 100 200 300 400 500 600 700 800 0 50 100 150 200 250 300 S h rin k a g e (m icr o -str a in s) Age (days) M30B M20R10B M20R10P1B R30B M35B M45B M35R10B PB MC-10 EC (b)
plain concrete (to maintain the workability of concrete after the addition of steel fibres) and
this may have led to more bleeding than in the other mixes. Overall, SFRC specimens
experienced higher amounts of average shrinkage strains compared to plain concrete,
possibly due to the air entrainment on the surface of the fibres. Shrinkage strains of SFRC
were between 500 and 600 micro-strains at the top and between 300 and 500 micro-strains at
the bottom. The scatter of the bottom measurements was higher than that of the top
measurements possibly due to the fact that the presence of steel fibres prevented some of the
coarse aggregates from settling to the bottom of the mould . The varying amounts of
coarse aggregates at the bottom of the section resulted in varying degrees of restrain and thus
a higher scatter in shrinkage resistance. Non-uniform shrinkage strains in these rectangular
sections can be the result of non-uniform distribution of the coarse aggregates across the
depth of concrete section, which also creates curvature that will contribute to the global
deformation of the members [25, 45].
3.1.2 Drying shrinkage and mass loss relationship
The relationship between total free shrinkage and mass loss of the CR specimens is
shown in Figure 4. Though the water content in the original mix was the same for all mixes,
workability decreased after introducing steel fibres as some of the free water was adsorbed in
wetting the surface of the fibres. Hence, it appears that, as a result, the plain concrete mix lost
more free water than the SFRC mixes during the first few days of drying.
The behaviour of each mix shows three stages: 1) the first five days of rapid drying, 2)
normal drying and 3) accelerated drying in the oven. The first stage indicates rapid mass loss
possibly due to the evaporation of the free water . The second stage tends to show a linear
trend in mass loss with free shrinkage until mass loss stabilises and the moisture inside the
samples become approximately equal to the relative humidity of the atmosphere . The
third stage was created artificially due to accelerated drying of the prisms in the oven initially
at 50 °C and then at 100 °C. During the first three cycles at 50 °C, there was little change in
mass loss and shrinkage. However, once the temperature was elevated to 100 °C, there was a
noticeable increase in mass loss and drying shrinkage.
Figure 4 Free shrinkage and mass loss relationship. 204
The purpose of completely drying the samples was to assess if it is possible to predict the
ultimate drying shrinkage strains from mass loss by assuming that the relationship between
shrinkage and mass loss is linear. However, during accelerated drying, there was more mass
loss (on average 14%) or less shrinkage (on average 19%) than expected under normal drying
conditions (second stage). This phenomenon may be attributed partly to micro diffusion of
water from gel pores to capillary pores, which helps to free larger amounts of water , or
to the micro-cracking that was caused by differential temperature at the surface of the
concrete during cooling. This was evident in the plain concrete that showed the highest
number of micro-cracks on the surface. Therefore, heating the samples at 100 °C appears to
have altered the mechanism of drying due to micro diffusion of water or micro-cracking,
which was not intended by the experiment. However, the ultimate mass loss could be
obtained at lower temperatures, e.g. at about 80 °C without causing damage in the concrete
micro-structure, and could be used to predict the long-term evolution of drying shrinkage
strain and its impact on the health of the structure.
3.1.3 Humid concrete shrinkage strains
Figure 5 shows the evolution of shrinkage strain in specimens conditioned in a mist
room. Negative strain values mean that the samples are swelling. The non-uniformity in the
curves between age of 50 and 70 days was due to unexpected fluctuations in moisture inside
the mist room (due to some mechanical problems). The initial swelling in the samples can be
attributed to swelling in GGBS grains, which can absorb water and lead to disjointing
pressure [48, 49], as they get fully saturated during the hydration process. As a result,
swelling continues until the relative humidity in the matrix becomes less than the relative
humidity in the pores of the grains . However, the plain concrete specimens swelled less
compared to those reinforced with fibres, possibly due to their lower permeability, which
prevented the GGBS in the matrix from absorbing any additional water .
Swelling continued for the entire 11-month period of measurements, which indicates that
swelling due to absorption of moisture is higher than any autogenous shrinkage strains.
Model B3  and fib MC-2010  predict expansion in any concrete stored under relative
humidity of about 100%. Predictions by model B3 and fib MC-2010 are shown in dashed
lines in Figure 5 (indicated as B3 and MC, respectively). B3 is found to be in agreement with
the initial experimental results while MC is close to the plain concrete throughout the
measuring period. It should be noted that this analysis was carried out using CEM I as a
cementitious material in both models as there is no provision for GGBS in the current
formulations. fib MC-2010 was found to predict expansion strains up to two times greater
than those induced by autogenous shrinkage strains.
Figure 5 Humid concrete strain results. 242
3.2 Restrained shrinkage strains
Figure 6 (a and b) shows the restrained shrinkage strains of all tested prism at the top (T)
and bottom (B), respectively. In general, prisms made with different mixes exhibited similar
restrained shrinkage strain development, apart from those made with mixes M35 and R30,
which started deviating from the rest between the age of 14 and 28 days. No significant
development in shrinkage took place in mix M35, possibly due to early age micro-cracking
near the anchors, whilst there was a remarkable increase in mix R30, possibly due to slip at
the interface between concrete and anchors.
Shrinkage strains varied between 250 and 300 micro-strains at the top and between 160
and 180 micro-strains at the bottom at the age of 180 days. These strains decreased after 200
days, possibly as a result of creep and the development of micro-cracks inside the concrete.
The similarity in the shrinkage strain levels exhibited by all specimens indicates that the
effect of steel fibre type and dosage is insignificant with respect to restrained shrinkage, as
was also observed in free shrinkage prisms. It should be noted that some of the curvature
induced in the specimens can be attributed to restraint loss at the external boundaries between
the concrete and steel anchors and/or differential aggregate distribution.
258 -150 -100 -50 0 50 0 50 100 150 200 250 300 350 S h rin k a g e (m icr o -str a in ) Age (days) M30 M35 M45 M20R10 M35R10 R30 M20R10P1 P B3 MC
Figure 6 Restrained shrinkage strains at top (a) and bottom (b). 259
3.3 Performance of the restraining frame
The degree of restraint (DOR) is defined as the difference in strain between the free and
restrained elements (see Equation (1)). The DOR values for the passive restraining frame
used varied between 0.5 and 0.6. The theoretical values using simple elastic calculations is
264 higher at 0.73 . 265 0 50 100 150 200 250 300 350 400 0 50 100 150 200 250 300 S h rin k a g e (m icr o -str a in s) Age (days) M30T M20R10T M20R10P1T R30T M35T M45T M35R10T (a) 0 50 100 150 200 250 300 350 400 0 50 100 150 200 250 300 S h rin k a g e (m icr o -str a in s) Age (days) M30B M20R10B M20R10P1B R30B M35B M45B M35R10B (b)
Drying shrinkage induces shortening of the concrete specimens, which are restrained by
the frame through the anchors. Figure 7 shows that there is some additional deformation at
the boundaries between concrete and the restraining frame over a gauge length of 100 mm
(see Figure 1c) for a typical mix (M20R10P1) at the top (T) and bottom (B) of each specimen
(1 - top, 2 - middle and 3 - bottom prism in the restraining frame). The deformations are
higher at the top of prisms 2 and 3 whilst they are similar for all prisms at the bottom level.
Most of the deformation takes place during the first 50 days. This deformation is the result of:
a) elastic deformation of the concrete, b) anchor elongation, c) slip at the interface between
concrete and anchors and d) local deformation of the frame. These additional deformations
b), c) and d) contribute to the differences between the actual (0.57) and theoretical (0.73)
Figure 7 Deformation at the boundary between restraining frame and concrete specimens, mix M20R10P1. 278
A numerical investigation was conducted by Younis (2014)  using 3D linear FEA
models in ABAQUS  to estimate the induced deformations by concrete drying shrinkage
on the restraining frame. Solid (continuum) elements with 8 integration points (CD8R) were
used. The approximate global mesh size was 20 mm, but a finer mesh was adopted close to
283 0.00 0.02 0.04 0.06 0.08 0.10 0 50 100 150 200 250 300 De fo rm a tio n (m m ) Age (days) 1T 2T 3T 1B 2B 3B
the connections. The model was run without the presence of concrete elements and
stressing forces on the rods inside the square hollow sections (SHS). This study adopted this
model, but modified the boundary conditions, modelling of concrete prisms and pre-stressed
forces as follows; the right column (CS) was fixed (welded) to the SHSs and to the base of
the frame whilst the left CS was pinned by pre-stressed forces of 56.25 kN (the result of a
torque of 180 N.m on the bolts) applied to rods inside the SHS. The anticipated induced force
due to dr ing shrinkage ( shEcAc), at the age of 300 days, was applied uniformly on the
anchors. At this age, the specimens have reached hygral stabilisation and the relative
deformation between concrete and frame can be considered to be approximately stabilised
(see Figure 7). Therefore, the shrinkage induced force can be assumed to be 100% resisted by
Figure 8 shows the exaggerated global and local deformations of the restraining frame
obtained by FEA. Concrete shrinkage caused relative translation of the CS and bending in
both CS and SHS. The relative translation between the columns at the level of prism 1, 2 and
3 is 0.127, 0.075 and 0.087 mm, respectively, corresponding to RF of 0.64, 0.79 and 0.75.
The bending deformation of the SHS restraining prism 1 is higher than that at prisms 2 and 3
due to the free end effect. Prism 2 experienced the lowest deformations due to the restraint
contribution of both top and bottom SHSs. Figure 8b shows the local deformation of the CS
at the level of prism 2 and the relative deformation between web and flanges. This highlights
the additional contribution to the boundary zone deformation due to local deformations of the
frame, which can actually account for some of the deformation shown in Figure 7. Much of
this local deformation can be avoided if the CS is locally stiffened to prevent the flange
rotation. The average apparent measured RF at 300 days was 0.57 whilst the theoretical and
numerical DORs are very similar at 0.73.
Figure 8 Exaggerated global and local deformation in the restraining frame (a) and supporting column (b). 309
4. Results and Discussion on Mechanical Characteristics
4.1 Compressive strength
Table 3 shows the average results of density and compressive strength for the plain
concrete mixes, for both air and water cured cubes (standard deviations are shown in
parenthesis). For air cured cubes, there was only a slight increase in the compressive strength
between 7 and 28 days whereas for water cured specimens, there was a dramatic change in
compressive strength due to the activation of the GGBS in the presence of water. The GGBS
is also responsible for the lower in early strength of the water cured samples at 7 days [35,
53]. At 14 months, the compressive strength for the samples stored in air is similar to that
measured at 28 days, while there was an increase from 40 MPa to 56 MPa for the water cured
Table 3 Plain concrete density and compressive strength results (standard deviation). 322
Density (kg/m3) Compressive Strength (MPa)
7 days 28 days 14 months 7 days 28 days 14 months
Water Cured 2387 (11) 2415 (16) 2405 (29) 22.6 (0.6) 40.1 (0.2) 56.0 (1.2)
Figure 9 shows the mean compressive strength values, obtained from three cubes (150
mm) per mix at 35 and 105 days (moisture cured in the laboratory) as well as from six
samples for each curing condition (MR, CR, RS) obtained from the broken prisms in flexure
at the age of 14 months. At age of 14 months, SFRC obtained from broken prisms shows
higher compressive strength compared to plain concrete at the same curing condition.
However, in all cases, the dose of the steel fibres appears to have no clear effect on
As expected, prisms stored in the mist room (MR) show much higher compressive
strength compared to the ones air cured in the control room (CR and RS) by about 56% on
average. CR and RS samples resulted in similar compressive strengths despite the fact that
RS samples were restrained for ten months and experienced drying shrinkage micro-cracks.
This may be because CR samples were fully dried in an oven (to determine mass loss) which
may have caused micro-cracks and weakened their structure. Micro-cracks were observed on
the surface of plain concrete specimens as discussed in subsection 3.1.2.
Figure 9 Compressive strength obtained from cubes at 35 and 105 days and broken prisms in flexure at 14 months. 339 0 10 20 30 40 50 60 70 80 C o m p ress iv e Stre n g th ( MP a)
4.2 Flexural Performance
Figure 10 (a-f) shows the stress-CMOD results (average of three prisms) for specimens
conditioned in MR, CR and RS environments. The initial elastic behaviour of all specimens,
shown in the graphs up to CMOD of 0.2 mm, is very similar. This confirms that the test
arrangement and measuring method is accurate and reliable and that the fibre content does
not influence much the elastic modulus. The plain concrete mix (P) shows the lowest strength
and least overall toughness. The fibre content seems to have some influences on residual
tensile strength with some mixes (e.g. CR M35) showing up to 100% increase in strength and
clear strain hardening characteristics. The initiation of cracking in the plain concrete appears
to take place just before the peak load at a CMOD of 0.02 mm. The same applies to all other
specimens and, as expected, fibres get mobilised and control the crack development. In
several cases, there is some initial drop in stress after the opening of the crack at around 0.03
mm until the fibres are mobilised sufficiently and contribute to stiffening the cracked
concrete. Sudden drops in stress are also seen in the post-peak range, due to fibre fracture or
All prisms conditioned in the mist room (MR) show higher strength and toughness than
the CR specimens by about 40% on average. This highlights the importance of curing in
strength development as well as the dominance of concrete strength on the flexural strength
of SFRC. Higher concrete strength also results into higher bond strength between the
concrete and fibres, which contributes to higher toughness. However, this also leads to more
fibres fracturing during the post-peak stage than slipping, as indicated by the fracturing
sounds during the test. In the case of the MR conditioned specimens (see Figure 10b), the
higher concrete strength leads to a high flexural strength when the first crack develops, but
due to high bond, more fibres break, leading to mainly flat post-cracking behaviour. On the
other hand, CR and RS conditioned specimens, which have a lower concrete strength, show a
lower flexural strength at first crack, but mobilize more fibres due to slippage, which leads to
smoother curves with hardening behaviour [54, 55].
367 M R -St res s ( MPa ) C R -Str es s (MP a) RS -Str es s (MP a) CMOD (mm) CMOD (mm)
Figure 10 Stress-CMOD curves a) MR-0.2 mm, b) MR, c) CR-0.2 mm, d) CR e) RS-0.2 mm, f) RS. 368
4.3 Residual flexural tensile strength
This sub-section examines the effect of fibre type and dosage, curing and restrain
condition on the flexural strength at the limit of proportionality (fLOP) and residual flexural 371 M30 M35 M20R10 M45 M20R10P1 M35R10 R30 P
tensile strength values (fR1, fR2, fR3, fR4) at different CMODs (0.5 mm, 1.5 mm, 2.5 mm and 372
3.5 mm). In accordance to EN 14651:2005, fLOP is taken as the maximum stress value up to 373
CMOD of 0.05 mm.
4.3.1 Effect of curing
Figure 11 (a and b) shows the change in flexural strength and residual values for the
specimens subjected to different conditions (MR and RS) relative to the CR condition. Figure
11a shows that mist curing increases fLOP by up to 90% (on average 60%), but this increase 378
decreases at larger CMODs. This confirms that curing has a significant effect on concrete
strength development as reflected by the increase in fLOP. However, as the effect on fR values 380
reduces with increasing CMOD, curing condition has less impact on the bridging capacity of
fibres which, at large CMOD, depends more on frictional stresses, geometrical characteristics
and less on bond strength.
Figure 11 Change in flexural and residual flexural tensile strength relative to CR in a) MR and b) RS. 384 -20 0 20 40 60 80 100 fLOP fR1 fR2 fR3 fR4 Ch an g e (% ) (a) MR -60 -40 -20 0 20 40 fLOP fR1 fR2 fR3 fR4 Ch an g e (% ) M30 M20R10 M20R10P1 R30 M35 M45 M35R10 (b) RS
4.3.2 Effect of restraint
Figure 11b shows the relative change in flexural strength due to restraint. The figure
shows an overall loss of fLOP on average of 10% due to restraint, despite the fact that no 388
cracks were visible on the RS specimens. However, as tensile strain and stress developed in
the RS specimens, micro-cracking must have taken place and caused some damage to the
concrete. The effect of the damage and micro-cracks appears to overall increase marginally as
the CMOD increases. Specimens manufactured with mix R30 show better performance partly
because they were not well restrained, thus could lead to smaller cracks that self-healed.
healing in restrained concrete was also reported by Younis (2014) .
4.3.3 Effect of fibres
Figure 12 (a-c) shows the change in flexural strength and residual flexural tensile stresses
due to the substitution of MUSF with RTSF for a total fibre content of 30 kg/m3 under MR,
CR and RS conditions, respectively. The changes are shown relative to M30 for each
respective condition. In Figure 12a, the effect of substituting MUSF with 10 kg/m3 of RTSF
results in about 10% reduction in both fLOP and residual flexural tensile stresses, as this 400
substitution did not affect much the concrete tensile strength and concrete-fibre interface
bond strength. In larger specimens (150 mm prisms and slabs), the blends with 10 kg/m3
RTSF showed a positive change in fLOP and fR values . This can be attributed to the fact 403
that fibre alignment is more critical in cast elements with small cross section due to boundary
effect, thus a small reduction in the amount of MUSF (which is longer) can affect
significantly the post cracking behaviour. The highest strength reduction at bigger CMODs
was observed in specimens made with mix R30, partly due to fibre slippage as RTSF have
shorter and thinner geometries compared to MUSF and partly due to their more random
distribution. The reduction in fLOP for specimens conditioned in CR (Figure 12b) is higher 409
than that found in MR samples by about 20%, but this may be more to do with the high fLOP 410
values of M30 than the effect of fibres, as the fR values changes are similar to those observed 411
for MR samples (Figure 12a).
When the concrete is restrained (see Figure 12c), even though there is an overall drop in
fLOP of 10%, the fibres do not appear to influence fLOP. However, there is a drop of about 30% 414
in the fR values of the blended mixes and of about 40% for the R30 mix. This is possibly due 415
to the reasons given above to Figure 12a.
416 -70 -60 -50 -40 -30 -20 -10 0 10 fLOP fR1 fR2 fR3 fR4 Ch an g e (% ) (a) -70 -60 -50 -40 -30 -20 -10 0 10 fLOP fR1 fR2 fR3 fR4 Ch an g e (% ) (b)
Figure 12 Change in residual flexural tensile strength due to substitution of MUSF with RTSF conditioned in a) MR, b) CR and 417
c) RS. 418
4.4 Characteristic residual flexural tensile strength ratios
In order to replace parts of conventional reinforcement with fibres in concrete structures,
fib MC-2010 imposes that the minimum values of characteristic residual flexural tensile
strength ratios at serviceability (fR1k/fLk) and ultimate limit state (fR3k/fR1k) conditions, be 0.4 422
and 0.5, respectively (fLk, fR1k and fR3k are the characteristic values at fLOP, fR1 and fR3, 423
respectively). These characteristic values are calculated using RILEM TC 162-TDF (2003)
 and depend on the number of specimens tested per parameter.
Figure 13 shows the serviceability characteristic residual flexural tensile strength ratios
(fR1k/fLk) for all mixes in MR, CR and RS conditions. Mixes with a total of 30 kg/m3 of steel 427
fibres show ratios less than one, while mixes with a total of 45 kg/m3 show ratios mostly
greater than one. Mixes with 45 kg/m3 contain considerably more longer manufactured fibres
which have a larger diameter and can resist tension more effectively even at larger CMOD.
CR and RS specimens with a total fibre content more than 35 kg/m3 have higher ratios than
MR specimens, due to their lower fLOP. 432 -70 -60 -50 -40 -30 -20 -10 0 10 fLOP fR1 fR2 fR3 fR4 Ch an g e (% ) M30 M20R10 M20R10P1 R30 (c)
Figure 13 Ratio of characteristic strength, fR1k/fLk. 434
Figure 14 shows the ultimate characteristic residual flexural tensile strength ratios
(fR3k/fR1k) for all specimens subjected to MR, CR and RS conditions. Most of fR3k/fR1k ratios 437
for the CR and RS specimens are greater than those for MR samples. This can again be
attributed to the higher fLOP achieved in the MR samples as a result of better curing. Overall, 439
all blends satisfied the required ratios of fib MC-2010 for serviceability and ultimate limit
states. Hence, blends of MUSF and RTSF can be used to replace part of conventional
reinforcement in RC structures.
Figure 14 Ratio of residual characteristic strength, fR3k/fR1k. 444 445 0.0 0.5 1.0 1.5 2.0 fR1k /fR L k MR CR RS 0.0 0.5 1.0 1.5 2.0 fR3k /fR 1k MR CR RS
This paper presents the free and restrained shrinkage behaviour of FRC specimens with
different fibre type (MUSF, RTSF and various blends) and their associated mechanical
characteristics. It has been shown that the utilisation of GGBS and RTSF in concrete mixes
contributes to reducing shrinkage strains and controlling cracking. Based on the experimental
results the following conclusions can be drawn:
Free shrinkage was much lower than predicted by the design codes by 35% on
average due to the use of GGBS.
Non-uniform shrinkage strains through the height of plain and SFRC sections were
observed in free and restrained elements, possibly due to uneven distribution of coarse
Average shrinkage strains in SFRC were higher than in plain concrete, possibly due to
an increase in air voids.
Drying and end restraint caused the development of micro-cracking in the concrete
which resulted in lower compressive strength (by about 56% on average) and residual
flexural tensile strength (up to 40%).
Curing has a significant effect on concrete strength development, but less impact on
the bridging capacity of fibres which depends more on frictional stresses.
The high residual flexural tensile strength of SFRC (cured in MR) and the high
frictional stresses between the concrete and the fibres caused the used small dosages
of fibres to break, due to the highly applied tensile stress on fibres.
The decay in the stress-CMOD curves show that the hybrid mixes of MUSF and
RTSF satisfy the ratios imposed by the fib MC-2010 and can reduce the required
amount of conventional reinforcement in concrete structures.
The researchers are gratefully acknowledging the financial support provided by the EC
collaborative FP7-ENV-2013-two-stage project "ANAGENNISI - Innovative Reuse of All
Tyre Components in Concrete" under grant number 603722 and the Omani government for
sponsoring the first author. We also appreciate the technical support provided by the
postgraduate students and engineering technicians in the concrete laboratory.
 ACI- R R E -A C C M M A
Concrete Institute, Farmington Hills, 2010.
 N B B F M “ C
-Construction and Building Materials, vol. 44, p. 249 259, 2013.
 N B C Y “ M R “ C ng in Fiber Reinforced Concrete:
A N T T Cement and Concrete Research, vol. 26, no. 1, pp. 9-14, 1996.
 K H Y R T
University of Sheffield, Sheffield, 2014.
 ) ) L L J B R “ F R C
Construction and Building Materials, vol. 85, p. 195 207, 2015.
 D.-Y. Yoo, Y.-“ Y N B P -cracking behavior of normal- and high-strength steel-fiber- Construction and Building Materials, vol. 93, p. 477 485, 2015.  M B D D J K I D A B P wi D  A K D A F D L R E Materials and Design, vol. 63, p. 493 499, 2014.  E M A C H X A -cracking behaviour
of Hybrid Industrial/Recycled Steel Fibre-R C Construction and Building Materials, vol. 94, p. 290 298, 2015.
 “ Y G I V T E
“FRC Construction and Building Materials, vol. 21, p. 1250 1253, 2007.
 G. Chanvillard and P.-C A P -O B C “ F Advn Cem Bas Mat, vol. 4, pp. 28-41, 1996.
 K H Y K P A P -Restrained Shrinkage Mechanical Properties
C ACI MATERIALS JOURNAL, vol. 113, no. 3, pp. 267-276, 2016.
 G C M L M A “
A Construction and Building Materials, vol. 36, pp.
 N. Jafarifar, “ B “ F R C P T
University of Sheffield, Sheffield, 2012.
 Â G G L -term performance of recycled steel fibre reinforced concrete for pavement
T U Sheffield, Sheffield, 2011.
 B A M A T M
reinforced self- Construction and Building Materials, vol. 28, p. 287 293, 2012.
 H. Hu, P. Papaste H A M G K P F
 A C H X P F E M E merical characterization
of the bond behavior of steel fibers recovered from waste tires embedded in cementitious Cement & Concrete Composites, vol. 62, p. 146 155, 2015.
 O “ M l fibers recovered from
Construction and Building Materials, vol. 122, pp. 649-658, 2016.
 W ) Y H “ H N D
incorporating ground granulated blast furnace sla
Construction and Building Materials, no. 93, pp. 267-277, 2015.
 K ) “ M “ E “ “ -compacting Concrete
C M M M
 D W H I A R “ C ACI Journal, pp.
 R I G “ C D “ C “
Electronic Journal of Structural Engineering, vol. 1, pp. 15-37, 2001.
 M H R B B C A “ H C
ACI Materials Journal, vol. 86, no. 2, pp. 185-190, 1989.
 J.-H. Jeong, Y.-S. Park and Y.-H L V “ inkage Strain within the Depth of Concrete
B Materials, pp. 7780-7794, 2015.
Materials and structures, vol. 31, pp. 507-512, 1998.
 A C “ J F T N J G “ R I G C
C Materials and Structures, vol. 49,
no. 5, p. 1619 1628, 2016.
 A. M. Neville, Properties of Concrete, Fourth ed., London: Pearson Education Limited, 2004.
 I G C - D
 M G “ P “ “ C F R C ACI Materials
Journal, vol. 87, no. 2, pp. 138-148, 1990.
 H C M L R K T N G K R
Construction and Building Materials, vol. 84, p. 468 476, 2015.
 R B A B F R “ N H -Strength
C ACI Materials Journal, vol. 92, no. 2, pp. 211-217, 1995.
 A M P M B J J “ E F A on on the Autogenous Shrinkage of
“ F C ACI Materials Journal, vol. 86, no. 2, pp. 139-144, 1989.
 “ A D L C
ACI Materials Journal, vol. 98, no. 4, pp. 323-331, 2001.
 T A J G “ “
-Magazine of Concrete Research, vol. 1, no. 60, pp. 41-48, 2008.
 A L P L R L “ “CC The influence of paste volume
Construction and Building Materials, vol. 25, no. 5, pp. 2283-2289, 2011.
 R L A L “ nkage cracking of self-compacting
Materials and Structures, no. 42, pp.
 EN- T - Measuring the flexural tensile strength
(limit of pr LOP E C “ B
 BSI- T - BS 1881 Part 119: Method for determination of compressive strength using portions of beams broken in flexure (equivalent cube method B B“I London, 1998.
 H H P P H A M G K P M
“FRC U Construction
and Building Materials, no. 163, pp. 376-389, 2018.
 CEN E D P -1: General rules and rules for Structures
 M C C “ W E & Sohn, Berlin, Germany,
 L J Y Y A
Cement and Concrete Research, no. 31, pp. 1203-1206, 2001.
 W M C A T age-reducing-admixture with ground,
granulated, blast- UCL D C
Environmental and Geomatic Engineering, London, 2015.
 Z. Al-K M G K P N -uniform drying shrinkage of RC elements
 R D T F K G M A “ G L E F
Cement & Concrete
Composites, vol. 27, no. 5, pp. 537-546, 2005.
 ) P B “ B C “ P M A D
C “ M B ACI M
 B. Craeye, G. D. Schutter, B. Desmet, J. Vantomme, G. Heirman, L. Vandewalle, Ö. Cizer, S.
A E K E -compacting
Cement and Concrete Research, no. 40, p. 908 913, 2010.
 A L P L C “ “CC Mechanical Properties of Self-Compacting Concrete, K. Khayat and G. (. De Schutter, Eds., Springer International Publishing, 2014, pp. 73-94.
 D “ O J N D B T fluence of superabsorbent polymers on the autogenous shrinkage properties of cement pastes with supplementary cementitious
Cement and Concrete Research, no. 74, pp. 59-67, 2015.
 M B A lity characteristics of steel fibre
Cement Combinations for Durable Concrete, Dundee, 2005.
 ABAQU“ “ D V “IMULIA D “ RI U“A
 C A C C C T
 A P F H M P V M
-Cement and Concrete Research, vol. 39, p. 1217 1229, 2009.
 K. Wille, S. El-T A N P
reinforced concrete (UHP-FRC Cement & Concrete Composites, vol. 48, pp. 53-55, 2014.
 RILEM-TC-162-TDF RILEM TC -TDF: Test and design methods for steel fibre reinforced Materials and Structures, vol. 36, pp. 560-567, 2003.